# Micromagnetic Simulations of Chaotic Ferromagnetic Nanofiber Networks

^{1}

^{2}

^{*}

## Abstract

**:**

## 1. Introduction

## 2. Simulations

_{S}= 1700 × 10

^{3}A/m, exchange constant A = 21 × 10

^{−12}J/m, magneto-crystalline anisotropy constant K

_{1}= 48 × 10

^{3}J/m

^{3}. The Gilbert damping constant was set to α = 0.5 (equivalent to a quasi-static case).

^{−11}J/m, magnetic polarization at saturation J

_{s}= 1 T, and the Gilbert damping constant α = 0.01.

## 3. Results and Discussion

_{x}) and along the z-axis (M

_{z}).

## 4. Conclusions

## Author Contributions

## Funding

## Conflicts of Interest

## References

- Pan, J.-F.; Liu, N.-H.; Sun, H.; Xu, F. Preparation and Characterization of Electrospun PLCL/Poloxamer Nanofibers and Dextran/Gelatin Hydrogels for Skin Tissue Engineering. PLOS ONE
**2014**, 9, e112885. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Grothe, T.; Wehlage, D.; Böhm, T.; Remche, A.; Ehrmann, A. Needleless Electrospinning of PAN Nanofibre Mats. Tekstilec
**2017**, 60, 290–295. [Google Scholar] [CrossRef] - Maver, T.; Kurečič, M.; Smrke, D.M.; Kleinschek, K.S.; Maver, U. Electrospun nanofibrous CMC/PEO as a part of an effective pain-relieving wound dressing. J. Sol-Gel Sci. Technol.
**2015**, 79, 475–486. [Google Scholar] [CrossRef] - Grimmelsmann, N.; Grothe, T.; Homburg, S.V.; Ehrmann, A. Electrospinning and stabilization of chitosan nanofiber mats. IOP Conf. Ser. Mater. Sci. Eng.
**2017**, 254, 102006. [Google Scholar] [CrossRef] - Salalha, W.; Dror, Y.; Khalfin, R.L.; Cohen, Y.; Yarin, A.L.; Zussman, E. Single-Walled Carbon Nanotubes Embedded in Oriented Polymeric Nanofibers by Electrospinning. Langmuir
**2004**, 20, 9852–9855. [Google Scholar] [CrossRef] - Lim, J.-M.; Moon, J.H.; Yi, G.-R.; Heo, C.-J.; Yang, S.-M. Fabrication of One-Dimensional Colloidal Assemblies from Electrospun Nanofibers. Langmuir
**2006**, 22, 3445–3449. [Google Scholar] [CrossRef] - Na, K.-H.; Kim, W.-T.; Park, D.-C.; Shin, H.-G.; Lee, S.-H.; Park, J.; Song, T.-H.; Choi, W.-Y. Fabrication and characterization of the magnetic ferrite nanofibers by electrospinning process. Thin Solid Films
**2018**, 660, 358–364. [Google Scholar] [CrossRef] - Döpke, C.; Grothe, T.; Steblinski, P.; Klöcker, M.; Sabantina, L.; Kosmalska, D.; Blachowicz, T.; Ehrmann, A. Magnetic Nanofiber Mats for Data Storage and Transfer. Nanomaterials
**2019**, 9, 92. [Google Scholar] [CrossRef] [Green Version] - Ryu, K.-S.; Thomas, L.; Yang, S.-H.; Parkin, S.S.P. Current Induced Tilting of Domain Walls in High Velocity Motion along Perpendicularly Magnetized Micron-Sized Co/Ni/Co Racetracks. Appl. Phys. Express
**2012**, 5, 093006. [Google Scholar] [CrossRef] - Yang, S.-H.; Ryu, K.-S.; Parkin, S. Domain-wall velocities of up to 750 m s
^{−1}driven by exchange-coupling torque in synthetic antiferromagnets. Nat. Nanotechnol.**2015**, 10, 221–226. [Google Scholar] [CrossRef] - Alejos, O.; Raposo, V.; Sánchez-Tejerina, L.; Martínez, E. Efficient and controlled domain wall nucleation for magnetic shift registers. Sci. Rep.
**2017**, 7, 11909. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Garg, C.; Yang, S.-H.; Phung, T.; Pushp, A.; Parkin, S.S.P. Dramatic influence of curvature of nanowire on chiral domain wall velocity. Sci. Adv.
**2017**, 3, e1602804. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Blachowicz, T.; Ehrmann, A. Magnetization reversal in bent nanofibers of different cross sections. J. Appl. Phys.
**2018**, 124, 152112. [Google Scholar] [CrossRef] [Green Version] - Kern, P.; Döpke, C.; Blachowicz, T.; Steblinski, P.; Ehrmann, A. Magnetization reversal in ferromagnetic Fibonacci nano-spirals. J. Magn. Magn. Mater.
**2019**, 484, 37–41. [Google Scholar] [CrossRef] - Wang, Z.; Crandall, C.; Sahadevan, R.; Menkhaus, T.; Fong, H. Microfiltration performance of electrospun nanofiber membranes with varied fiber diameters and different membrane porosities and thicknesses. Polymer
**2017**, 114, 64–72. [Google Scholar] [CrossRef] - Yalcinkaya, F.; Hruza, J. Effect of Laminating Pressure on Polymeric Multilayer Nanofibrous Membranes for Liquid Filtration. Nanomaterials
**2018**, 8, 272. [Google Scholar] [CrossRef] [Green Version] - Tripathy, M.; Hota, G. Maghemite and Graphene Oxide Embedded Polyacrylonitrile Electrospun Nanofiber Matrix for Remediation of Arsenate Ions. ACS Appl. Polym. Mater.
**2019**, 2, 604–617. [Google Scholar] [CrossRef] - Fokin, N.; Grothe, T.; Mamun, A.; Trabelsi, M.; Klöcker, M.; Sabantina, L.; Döpke, C.; Blachowicz, T.; Hütten, A.; Ehrmann, A. Magnetic Properties of Electrospun Magnetic Nanofiber Mats after Stabilization and Carbonization. Materials
**2020**, 13, 1552. [Google Scholar] [CrossRef] [Green Version] - Bica, I.; Anitas, E.M.; Choi, H.; Sfirloaga, P. Microwave-assisted synthesis and characterization of iron oxide microfibers. J. Mater. Chem. C
**2020**. [Google Scholar] [CrossRef] - Petropoulou, A.; Kralj, S.; Karagiorgis, X.; Savva, I.; Loizides, E.; Panagi, M.; Krasia-Christoforou, T.; Riziotis, C. Multifunctional Gas and pH Fluorescent Sensors Based on Cellulose Acetate Electrospun Fibers Decorated with Rhodamine B-Functionalised Core-Shell Ferrous Nanoparticles. Sci. Rep.
**2020**, 10, 1–14. [Google Scholar] [CrossRef] - Wang, Y.J.; Sun, Y.; Zong, Y.; Zhu, T.G.; Zhang, L.X.; Li, X.H.; Xing, H.N.; Zheng, X.L. Carbon nanofibers supported by FeCo nanocrystals as difunctional magnetic/dielectric composites with broadband microwave absorption performance. J. Allows Compd.
**2020**, 824, 153980. [Google Scholar] [CrossRef] - Pan, J.; Guo, H.; Wang, M.; Yang, H.; Hu, H.; Liu, P.; Zhu, H. Shape anisotropic Fe3O4 nanotubes for efficient microwave absorption. Nano Res.
**2020**, 13, 621–629. [Google Scholar] [CrossRef] [Green Version] - Bhugra, V.S.; Williams, G.V.M.; Chong, S.V.; Nann, T. Electrospun, oriented, ferromagnetic Ni1-xFex nanofibers. Front. Chem.
**2020**, 8, 47. [Google Scholar] [CrossRef] [PubMed] - Zambano, A.J.; Pratt, W.P. Detecting domain-wall trapping and motion at a constriction in narrow ferromagnetic wires using perpendicular-current giant magnetoresistance. Appl. Phys. Lett.
**2004**, 85, 1562. [Google Scholar] [CrossRef] [Green Version] - Nasirpouri, F.; Peighambari-Sattari, S.-M.; Bran, C.; Palmero, E.M.; Eguiarte, E.B.; Vazquez, M.; Patsopoulos, A.; Kechrakos, D. Geometrically designed domain wall trap in tri-segmented nickel magnetic nanowires for spintronics devices. Sci. Rep.
**2019**, 9, 9010. [Google Scholar] [CrossRef] - Abbas, N.; Wang, F.; Ren, H.; Liu, J.P.; Xia, W.; Du, J.; Zhao, G.; Zhang, J. Determination of interface layer effects on magnetic properties of nanocomposite magnets and exchange coupling between magnetic entities. Appl. Surf. Sci.
**2019**, 480, 454–462. [Google Scholar] [CrossRef] - Donahue, M.J.; Porter, D.G. OOMMF User’s Guide, version 1.0; National Institute of Standards and Technology (NIST): Gaithersburg, MD, USA, 1999. [Google Scholar]
- Ehrmann, A.; Blachowicz, T. Vortex and double-vortex nucleation during magnetization reversal in Fe nanodots of different dimensions. J. Magn. Magn. Mater.
**2019**, 475, 727–733. [Google Scholar] [CrossRef] - Blachowicz, T.; Döpke, C.; Ehrmann, A. Micromagnetic Simulations of Electrospun Nanofiber Networks; Works of the Institute of Engineering Materials and Biomedical Materials, Silesian University of Technology: Gliwice, Poland, 2019. [Google Scholar]
- Scholz, W.; Fidler, J.; Schrefl, T.; Suess, D.; Dittrich, R.; Forster, H.; Tsiantos, V. Scalable parallel micromagnetic solvers for magnetic nanostructures. Comput. Mater. Sci.
**2003**, 28, 366–383. [Google Scholar] [CrossRef] - Blachowicz, T.; Ehrmann, A. Fourfold nanosystems for quaternary storage devices. J. Appl. Phys.
**2011**, 110, 73911. [Google Scholar] [CrossRef] [Green Version] - Stoner, E.C.; Wohlfarth, E.P. A mechanism of magnetic hysteresis in heterogeneous alloys. Philos. Trans. R. Soc. London. Ser. A Math. Phys. Sci.
**1948**, 240, 599–642. [Google Scholar] [CrossRef] - Sabantina, L.; Rodríguez-Cano, M.Á.; Klöcker, M.; Mateos, F.J.G.; Hidalgo, J.J.T.; Mamun, A.; Beermann, F.; Schwakenberg, M.; Voigt, A.-L.; Rodríguez-Mirasol, J.; et al. Fixing PAN Nanofiber Mats during Stabilization for Carbonization and Creating Novel Metal/Carbon Composites. Polymers
**2018**, 10, 735. [Google Scholar] [CrossRef] [PubMed] [Green Version]

**Figure 1.**Magnetization reversal process in sample NF1 for an external magnetic field along 45° from “lower left” to “upper right” orientation. From Blachowicz et al. [29].

**Figure 2.**Thickness dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for sample NF1 under an angle of 0°.

**Figure 3.**Thickness dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for sample NF1 under an angle of 45° (see Figure 1).

**Figure 4.**Thickness dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for a sample NF1 under an angle of 90°.

**Figure 5.**Angle dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for sample NF1 with a thickness of 120 nm.

**Figure 6.**Thickness dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for sample NF2 under an angle of 0°.

**Figure 7.**Thickness dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for sample NF2 under an angle of 45°.

**Figure 8.**Thickness dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for sample NF2 under an angle of 90°.

**Figure 9.**Angle dependence of (

**a**) the longitudinal and (

**b**) the transverse hysteresis loops, simulated for sample NF2 with a thickness of 120 nm.

**Figure 10.**Angle dependence of the longitudinal and transverse hysteresis loops simulated for sample NF2 with a thickness of 120 nm.

**Figure 11.**Influence of neighboring fibers in different distances on the magnetization reversal process, simulated for an angle of 45° and a thickness of 120 nm. (

**a**) two neighboring fibers NF2, (

**b**) three neighboring fibers NF2, (

**c**) five neighboring fibers NF2, and (

**d**) two adjacent fibers NF1.

**Figure 12.**(

**a**) Definition of the axes, magnetization components, (

**b**) M

_{x}, and (

**c**) M

_{z}in the non-random case of 0° possible deviation of the fiber orientation from the z-orientation.

**Figure 13.**Fiber orientations used in the simulations for random angle ranges, depicted in steps of 10°: (

**a**) 10°, (

**b**) 20°, (

**c**) 30°, (

**d**) 40°, (

**e**) 50°, (

**f**) 60°, (

**g**) 70°, (

**h**) 80°, and (

**i**) 90°.

**Figure 14.**Hysteresis loops, simulated for an external magnetic field sweep along the x-axis and random angle ranges, depicted in steps of 10°: (

**a**) 10°, (

**b**) 20°, (

**c**) 30°, (

**d**) 40°, (

**e**) 50°, (

**f**) 60°, (

**g**) 70°, (

**h**) 80°, and (

**i**) 90°.

**Figure 15.**Hysteresis loops, simulated for an external magnetic field sweep along the z-axis and random angle ranges, depicted in steps of 10°: (

**a**) 10°, (

**b**) 20°, (

**c**) 30°, (

**d**) 40°, (

**e**) 50°, (

**f**) 60°, (

**g**) 70°, (

**h**) 80°, and (

**i**) 90°.

© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Blachowicz, T.; Döpke, C.; Ehrmann, A.
Micromagnetic Simulations of Chaotic Ferromagnetic Nanofiber Networks. *Nanomaterials* **2020**, *10*, 738.
https://doi.org/10.3390/nano10040738

**AMA Style**

Blachowicz T, Döpke C, Ehrmann A.
Micromagnetic Simulations of Chaotic Ferromagnetic Nanofiber Networks. *Nanomaterials*. 2020; 10(4):738.
https://doi.org/10.3390/nano10040738

**Chicago/Turabian Style**

Blachowicz, Tomasz, Christoph Döpke, and Andrea Ehrmann.
2020. "Micromagnetic Simulations of Chaotic Ferromagnetic Nanofiber Networks" *Nanomaterials* 10, no. 4: 738.
https://doi.org/10.3390/nano10040738